Total of Rejected = 156 / out of 2085

= 7.5 %

Summary Table

TEST Selection Criteria^{Specified}_{Limit}^{Mean}_{Value}^{No. of}_{Rejected}^{% of}_{Rejected}

Gain Voltage V. spread at G = 500 K < 20% ~ 11 % Dark Current D.C. at G = 500 K < 5 nA 0.43 nA 10 0.5 % Linearity at G = 10 K

Peak Anode Current that gives a 2% dev

> 10 mA 16.5 mA 3 0.1 %

Linearity at G = 50 K > 20 mA 44.0 mA 2 0.1 % Linearity at G = 100 K > 35 mA 74.3 mA 3 0.1 % Linearity at G = 500 K > 70 mA 93.5 mA 35 1.7 % Stability with Time % Deviation in 48 hours < 6 % 2.2 % 55 2.7 % Stability with bkgr. Current

% Shift for ΔIBG = 1μA < 5 % 1.7 % 48 2.3 %